Test: Casting Level - 2 - Mechanical Engineering MCQ

# Test: Casting Level - 2 - Mechanical Engineering MCQ

Test Description

## 20 Questions MCQ Test - Test: Casting Level - 2

Test: Casting Level - 2 for Mechanical Engineering 2024 is part of Mechanical Engineering preparation. The Test: Casting Level - 2 questions and answers have been prepared according to the Mechanical Engineering exam syllabus.The Test: Casting Level - 2 MCQs are made for Mechanical Engineering 2024 Exam. Find important definitions, questions, notes, meanings, examples, exercises, MCQs and online tests for Test: Casting Level - 2 below.
Solutions of Test: Casting Level - 2 questions in English are available as part of our course for Mechanical Engineering & Test: Casting Level - 2 solutions in Hindi for Mechanical Engineering course. Download more important topics, notes, lectures and mock test series for Mechanical Engineering Exam by signing up for free. Attempt Test: Casting Level - 2 | 20 questions in 30 minutes | Mock test for Mechanical Engineering preparation | Free important questions MCQ to study for Mechanical Engineering Exam | Download free PDF with solutions
Test: Casting Level - 2 - Question 1

### Wood flour is added to core sand to improve:

Detailed Solution for Test: Casting Level - 2 - Question 1
Wood flour is added to improve collapsibility of core.

Test: Casting Level - 2 - Question 2

### Which of the following sand ramming methods result into hardest layer at parting plane and around the pattern and less dense in top layers?

Detailed Solution for Test: Casting Level - 2 - Question 2
Jolting results in hardest layer at parting plane and around the pattern and less dense in top layer.

 1 Crore+ students have signed up on EduRev. Have you?
Test: Casting Level - 2 - Question 3

### Recess provided in the material for locating and positioning of cores is called as:

Detailed Solution for Test: Casting Level - 2 - Question 3
Recess is provided in the material for locating and positioning of core is called Core print.

Test: Casting Level - 2 - Question 4

Match the following according to the properties of moulding sand

List-I

a. Cohesiveness

c. Refractoriness

d. Collapsibility

List-II

i. Ability of breaking the mould with little force

ii. Ability to withstand higher temperature without losing strength

iii. Ability of bond formation of sand particles with other materials

iv. Ability to form bond between sand particles

Test: Casting Level - 2 - Question 5

Match the four basic elements of moulding sand with its percentage

Test: Casting Level - 2 - Question 6

Which one is true for strainer:

Detailed Solution for Test: Casting Level - 2 - Question 6
Strainer acts as a filter for separating the impurities present in molten metal.

Test: Casting Level - 2 - Question 7

The shape factor for a casting in the form of an annular cylinder of outside diameter 30 cm, inside diameter 20 cm and height 30 cm (correction factor, k = 1 ) will be:

Detailed Solution for Test: Casting Level - 2 - Question 7

L = height = 30cm

( D0- D1 )/2   divided by 2 as it is diameter

Test: Casting Level - 2 - Question 8

Match List-I (Type of casting) with List-II (Working principles) and select the correct answer using the codes given below the lists:

List-I

a. Die casting

b. Centrifugal casting

c. Centrifuging

d. Continuous casting

List-II

1. Molten metal is forced into the die under pressure

2. Axis of rotation does not coincide with axis of mould

3. Metal solidifies when mould is rotating

4. Continuously pouring molten metal into mould

Detailed Solution for Test: Casting Level - 2 - Question 8

In die casting molten metal is forced in to die made up of metal.

In centrifugal casting axis of rotation coincide with axis of mould.

In centrifuging, axis of rotation does not coincide with axis of mould.

Test: Casting Level - 2 - Question 9

The correct reasons for the occurrence of hot tear in casting among the following reasons will be:

i. Hindered contraction occurring immediately after metal has solidified

ii. Poor collapsibility of mould and core

iii. Too high pouring temperature

Test: Casting Level - 2 - Question 10

Directional solidification means:

Detailed Solution for Test: Casting Level - 2 - Question 10

Directional solidification means solidification near riser will be at end.

Progressive solidification means the solidification is starting from wall of casting and proceeding towards the center of casting.

*Answer can only contain numeric values
Test: Casting Level - 2 - Question 11

A steel slab casting of dimensions 30 cm x 30 cm x 6 cm with a side riser is to be casted horizontally into the mould. Using modulus method, the volume of the cylindrical riser is __________cm3

Detailed Solution for Test: Casting Level - 2 - Question 11

The dimensions of the slab = 30 cm x 30 cm x 6 cm

This can be considered as a long bar with a cross section of (30 x 6)cm2

MR = 1.2 Mc

D = 15.4 cm

= 2872.95 cm3

Test: Casting Level - 2 - Question 12

The rate of formation of thickness (in mm) of the metal skin frozen during solidification of pure zinc casting is found to be 2 times of square root of solidification time (in s). What will be the solidification time if thickness of the solid zinc casting is 16 mm?

Detailed Solution for Test: Casting Level - 2 - Question 12

Where T is thickness

At t = 0, T = 0 ⇒ C = 0

= 5.24 sec

Test: Casting Level - 2 - Question 13

In a gating design, sprue has an area 5.4cm2 , where the pouring basin meets the sprue, sprue length is 30 cm and desired molten metal flow rate is 900 cm3 /s. The area of the sprue at the bottom to avoid air aspiration effect is:

Detailed Solution for Test: Casting Level - 2 - Question 13

hc = 14.16 cm

From continuity equation

= 3.0578 cm2

*Answer can only contain numeric values
Test: Casting Level - 2 - Question 14

A cylindrical side riser is used for a sand casting mold. The casting itself is a rectangular plate with dimensions 7.5 x 12.5 x 2 cm3 . The solidification time for this casting is 1.6 min. The cylinder for the riser has a diameter to height ratio equal to 1. If the riser and casting are in same mold, then for a riser solidification time of 2 min, its dimension is __________ cm

Detailed Solution for Test: Casting Level - 2 - Question 14

Volume of plate = 7.5 x 12.5 x 2 = 187.5 cm3

Surface area of plate

= 2 x (7.5 x 12.5 + 7.5 x 2 + 12.5 x 2)

=267.5 cm2

Cm = 3.26 min/cm2

Now, we design the riser so that its solidification time is 2 min, using the same value of mold constant as they both are in the same mold.

Now, triser = 2 min (Given)

D = 4.699 cm

*Answer can only contain numeric values
Test: Casting Level - 2 - Question 15

The following data is observed for a casting process:

Mass of casting = 5000 kg

Density of metal = 8000 kg/m3

Pouring time = 10 sec

Efficiency factor = 0.9

The chock area of the casting is ___________mm2

Detailed Solution for Test: Casting Level - 2 - Question 15

= 0.01108595 m2

= 11085.95 mm2

Test: Casting Level - 2 - Question 16

A cast steel slab of dimension 30 x 20 x 5 cm3 is poured horizontally using a side riser. The riser is cylindrical in shape with diameter and height both equal to 12 cm. The freezing ratio of mould for Caine’s empirical equation is:

Detailed Solution for Test: Casting Level - 2 - Question 16

= 0.567

= 1.134

Test: Casting Level - 2 - Question 17

What is the modulus of a optimum side riser in the shape of square parallelopiped with side a:

Detailed Solution for Test: Casting Level - 2 - Question 17

Optimum riser ⇒ heat transfer is minimum ⇒

S.A is minimum

Surface area = 2a2 + 4ah = S.A

V = a2 x h

⇒ 4V = 4a3

⇒ V = a3

⇒ a2h =a3 ⇒ a = h

Test: Casting Level - 2 - Question 18

Following are the steps followed in a typical casting process:

i. Moulding

ii. Pattern making

iii. Melting and pouring

iv. Core making

v. Testing and inspection

vi. Fettling

The correct sequence of steps will:

Detailed Solution for Test: Casting Level - 2 - Question 18

Correct sequence of steps in casting is Pattern making ➝ core making ➝ mould making ➝ melting and pouring ➝ fettling ➝ testing and inspection.

Test: Casting Level - 2 - Question 19

In risering analysis, for finding the riser contribution, chills are used to:

Detailed Solution for Test: Casting Level - 2 - Question 19
In risering analysis, towards finding the riser contribution chills are used to increase riser contribution and increase edge distribution.

Test: Casting Level - 2 - Question 20

Which of the following statements are true with regard to the hot chamber and cold chamber die cast machine?

i. Hot chamber die casting machine has a furnace for melting and holding the metal

ii. High melting temperature alloys of nonferrous type are best to die cast in hot chamber machines

iii. In cold chamber machine, metal is ladled by hand from a nearly holding furnace

Information about Test: Casting Level - 2 Page
In this test you can find the Exam questions for Test: Casting Level - 2 solved & explained in the simplest way possible. Besides giving Questions and answers for Test: Casting Level - 2, EduRev gives you an ample number of Online tests for practice